MICROSTRUCTURE, THERMO-PHYSICAL, MECHANICAL AND Microstructure, thermo-physical, mechanical and wear
Embed Size (px)
Transcript of MICROSTRUCTURE, THERMO-PHYSICAL, MECHANICAL AND Microstructure, thermo-physical, mechanical and wear
Ceramics-Silikáty 62 (1), 15-30 (2018) www.ceramics-silikaty.cz doi: 10.13168/cs.2017.0041
Ceramics – Silikáty 62 (1) 15-30 (2018) 15
MICROSTRUCTURE, THERMO-PHYSICAL, MECHANICAL AND WEAR PROPERTIES OF IN-SITU FORMED BORON
CARBIDE – ZIRCONIUM DIBORIDE COMPOSITE #T. S. R. CH. MURTHY*, ****, SAIRAM ANKATA**, J. K. SONBER*, K. SAIRAM*, ****, KULWANT SINGH*,
A. NAGARAJ***, P. SENGUPTA*, ****, R. D. BEDSE*, SANJIB MAJUMDAR*, ****, VIVEKANAND KAIN*, ****
*Materials Group, Bhabha Atomic Research Centre, Mumbai, India **Dept. of Metallurgical and Materials Engineering, Indian Institute of Technology, Kharagpur, India
***Laser and Plasma Technology Division, Bhabha Atomic Research Centre, Mumbai, India ****Homi Bhabha National Institute, Mumbai, India
Submitted July 1, 2017; accepted October 20, 2017
Keywords: Boron Carbide, Microstructure, XRD, Electrical resistivity, Thermal conductivity, Wear resistance
Microstructure, thermos-physical, mechanical and wear properties of in-situ formed B4C–ZrB2 composite were investigated. Coefficient of thermal expansion, thermal diffusivity and electrical resistivity of the composite were measured at different temperatures up to 1000°C in inert atmosphere. Flexural strength was measured up to 900°C in air. Friction and wear properties have been studied at different loads under reciprocative sliding, using a counter body (ball) of cemented tungsten carbide (WC–Co) at ambient conditions. X-ray diffraction (XRD) and electron probe microanalysis (EPMA) confirmed the formation of ZrB2 as the reaction product in the composite. Electrical resistivity was measured as 3.02 × 10-4 Ω·m at 1000°C. Thermal conductivity measured at temperatures between 25°C and 1000°C was in the range of 8 to 10 W·(m-K)-1. Flexural strength of the composite decreased with increase in temperature and reached a value of 92 MPa at 900°C. The average value of coefficient of friction (COF) was measured as 0.15 at 20 N load and 10 Hz frequency. Increase of load from 5 N to 20 N resulted in decrease in COF from 0.24 to 0.15 at 10 Hz frequency. Specific wear rate data observed was of the order of 10-5 mm3·(N-m)-1. Both abrasive and tribo-chemical reaction wear mechanisms were observed on the worn surface of flat and counter body materials. At higher loads (≥ 10 N) a tribo-chemical reaction wear mechanism was dominant.
Boron carbide (B4C) is a potential material for heavy duty wear applications, cutting tools, armor and neutron absorbers in various types of nuclear reactors (Pressurized water reactor, boiling water reactor, fast breeder reactor and high temperature reactors), due to its high melting point, hardness, wear resistance, moderate electrical and thermal conductivity, chemical stability, retention of strength at elevated temperatures and high neutron absorption cross-section for both thermal and fast neutrons [1-15]. Important properties of boron carbide are listed in Table 1 [3,16]. Despite its combination of attractive properties, the usage of B4C is limited in real life due to difficulties in densification and susceptibility to brittle failure [3, 17]. Covalent bonding prevalent in B4C necessitates high sintering temperatures close to the melting point for achieving full dense compacts [3, 18, 19]. Significant improvement in densification was observed when particles of nanometer or submicron size are used for sintering . Alternative methods for obtaining full density with good mechanical/physical properties are summarized below. Continuous research on boron carbide based cera- mics has proven that suitable second phase addition helps
in achieving improved sintering behavior and mechanical properties [3, 19, 20]. Additions of reducing elements such as carbon, silicon and aluminum containing additi- ves such as SiC, Be2C, TiC, AlN enhance the sintering kinetics by removing the surface oxide layers of boron carbide (usually B2O3 layer is present on B4C particles, which hinders densification) [3, 17, 19]. Metallic additives (such as Fe and Cu) facilitate liquid phase sintering and thus help in achieving dense bodies at lower sintering temperatures [3, 19]. However, metallic additives are detrimental to the unique properties of the hard ceramics . Alternatively, addition of non-metallic sinter addi- tives such as oxides, nitrides, carbides, borides (such as AlN, BN, ZrB2, HfB2) can enhance the densification as well as mechanical/physical properties [3, 17-19]. Advanced sintering techniques like spark plasma sinte- ring or flash sintering also reported that full density can be achieved at lower sintering temperatures in a short span of holding time (10 to 15 minutes) [18, 21]. Oxide additions as sintering aids are particularly interesting due to the chemical instability of B4C with respect to many oxides [19, 22]. The resulting chemical reactions during sintering not only enhances the densifi- cation but also improves the thermo-mechanical and physical properties of dense bodies via the formation
Murthy T. S. R. Ch. , Ankata S., Sonber J. K., Sairam K., Singh K., Nagaraj A., Sengupta P., Bedse R. D., Majumdar S., Kain V.
16 Ceramics – Silikáty 62 (1) 15-30 (2018)
of reaction products such as carbides or borides [3, 19, 22, 23]. The in-situ reaction of B4C with Me oxides (Me = Ti, Zr, Cr, V, Hf, Eu, La, and Y) yielded high dense B4C based composites (B4C-MeB2 composites) at a lower sintering temperatures with improved mecha- nical properties compared to monolithic boron carbide [3, 19, 22, 23]. It is reported that TiO2 addition to B4C has helped to enhance the densification, due to the formation of sub-stoichiometric B4C by reactive sintering [19, 24]. This sub-stoichiometric compound is believed to enhan- ce the mobility of the constituents, resulting in higher sinterability [19, 24]. The reaction between HfO2 and B4C results in the formation of B4C-HfB2 composites with improved thermo-mechanical properties as compa- red to monolithic B4C . Sairam et al.  reported fully dense B4C-HfB2 composites obtained by in-situ reaction of B4C and 2.5 % HfO2 during hot pressing at a temperature of 1900°C and a pressure of 40 MPa (under vacuum). Similarly, it is reported that the addition of ZrO2 is beneficial for densification due to the formation of ZrB2 as a reaction product . Tribology studies on monolithic boron carbide, B4C–BN (hexagonal) composites and SiC–B4C–Si cer- mets have been reported in the literature [25-27]. The coefficient of friction of boron carbide has been reported as low as 0.03, but some reports recorded values up to 0.9 [25-27], depending on the load, surface chemical com- position, counter body material and humidity. During tribological tests, B4C undergoes oxidation, which results in the formation of B2O3, which further converts to a boric acid (H3BO3) film in the presence of sufficient humidity [25, 28-31]. Boric acid based films reduce the friction by forming a smooth friction surface at the interface, acting as lubricants due to their layered structure . There is a demand for wear resistant components, which are used in mechanical systems that involve high temperatures, heavy loads, aggressive environments and high velocities. Refractory metal borides, carbides and their composites are natural candidates for these tribo- logical applications due to their exceptional hardness, elastic modulus and thermal stability at elevated tem- peratures [32-38]. Among these, boron carbide is one of the potential materials for wear resistant applications
. However, difficulties in consolidation, poor fracture toughness and moderate oxidation resistance restrict the widespread use of B4C [1, 3]. Preparation of in-situ formed B4C composites containing ZrB2 appears as a viable solution to overcome the above limitations . Although in-situ formed B4C–ZrB2 composites were reported in literature, the detailed characterization with respect to microstructure, thermophysical, mechanical and wear properties are rather limited. It is believed that the presence of second phases, especially ZrB2, will be helpful to enhance the thermos-physical and mechanical properties of boron carbide. In this study, the microstructure, thermos-physical, mechanical and wear properties of in-situ formed B4C–ZrB2 composite are investigated. Microstructural characterization is carried out using a scanning electron microscope (SEM) with energy dispersive spectroscopy (EDS) and wavelength dispersive spectroscopy (WDS), i.e. electron probe microanalysis (EPMA). coefficient of thermal expansion (CTE), thermal diffusivity and electrical resistivity are measured up to 1000°C in an inert atmosphere. Flexural strength is measured up to 900°C in air. Friction and wear properties of this composite have been studied at different loads under reciprocative sliding, using a counter body (ball) of cemented tungsten carbide (WC–Co).
Starting materials and consolidation
Boron carbide (B4C: 78.5 % B, 19.5 % C, < 1 % O, 0.02 % Fe, 0.02 % Si; Vajrabor HP3.5, Bhukhanvala) and reactor grade zirconium oxide, ZrO2 (impurities: 600 ppm Fe, 300 ppm Ca, 150 ppm Ti, 100 ppm Cr, 100 ppm Hf; RG, Nuclear Fuel Complex) were used to prepare dense B4C-ZrB2 composite in the present study. The weighed quantities of 95 wt. % B4C and 5 wt. % ZrO2 powders were mixed in a turbo mixer (MXM-2, Insmart Systems) for 4 h. The particle size distribution (Figure 1a) of mixed powders was measured by laser diffraction (PSA 1064L, CILAS). The morphology of mixed pow- ders was examined by SEM (MV2300CT/100,